Standard Test Method for Electrochemical Measurement of Diffusible Hydrogen in Steels (Barnacle Electrode)Übersetzen
NORM herausgegeben am 1.6.2017
Bezeichnung normen: ASTM F1113-87(2017)
Ausgabedatum normen: 1.6.2017
Zahl der Seiten: 6
Gewicht ca.: 18 g (0.04 Pfund)
Land: Amerikanische technische Norm
Kategorie: Technische Normen ASTM
barnacle cell, current transients, diffusion, electrochemical, electrodes, high strength steels, hydrogen contact, hydrogen embrittlement, mobile hydrogen ,, ICS Number Code 25.220.20 (Surface treatment)
|Significance and Use|
4.1 The critical level of hydrogen in steels is that hydrogen which can build up to high concentrations at points of high triaxial stress causing embrittlement of the steel which can lead to catastrophic damage. This hydrogen can enter by various means, such as during pickling and electroplating. Means of reducing this hydrogen during processing are given in Specification and Practices and . It is still necessary, however, to know how effective these methods are. Though the ultimate reason for measuring this hydrogen is to relate it to embrittlement, this is not within the scope of this test method. As susceptibility to hydrogen embrittlement is a function of alloy type, heat treatment, intended use,and so forth, the tolerance for hydrogen must be determined by the user according to Method .
4.2 Though the actual hydrogen concentration is not determined in this test method, the current densities have been shown to be useful as an indication of relative hydrogen concentrations 4.3 This test method is applicable as a quality control tool for processing (such as to monitor plating and baking) or to measure hydrogen uptake caused by corrosion.
4.4 This test method is nondestructive; however, if there is a coating, it must be removed by a method which has been demonstrated to neither damage the steel nor introduce hydrogen to make the measurement.
4.5 This test method is also applicable to situations producing continuous hydrogen permeation, such as high pressure hydrogen cylinders or corrosion processes. The results, however, would require a different treatment and interpretation 4.6 This test method is also applicable to small parts, such as fasteners. The technique, procedure, and interpretation would, however, have to be altered.
4.7 Use of this test method on austenitic stainless steels and other face centered cubic (FCC) alloys would require different measurement times and interpretation of results because of differing kinetics.
4.8 This test method can be used on slightly curved surfaces as long as the gasket defines a reproducible area. The area calculation must, however, be changed.
1.1 This test method covers the procedure for measuring diffusible hydrogen in steels by an electrochemical method.
1.2 This test method is limited to carbon or alloy steels, excluding austenitic stainless steels.
1.3 This test method is limited to flat specimens to which the cell can be attached (see and ).
1.4 This test method describes testing on bare or plated steel after the plate has been removed (see ).
1.5 This test method is limited to measurements at room temperature, 20 to 25°C (68 to 77°F).
1.6 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
1.7 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
|2. Referenced Documents|
Wollen Sie sich sicher sein, dass Sie nur die gültigen technischen Normen verwenden?
Wir bieten Ihnen eine Lösung, die Ihnen eine Monatsübersicht über die Aktualität der von Ihnen angewandten Normen sicher stellt.
Brauchen Sie mehr Informationen? Sehen Sie sich diese Seite an.
Letzte Aktualisierung: 2018-07-18 (Zahl der Positionen: 2 043 698)
© Copyright 2018 NORMSERVIS s.r.o.